plasmonic nanopore with nanopattern and nanoparticles for single molecule 2018-03-02آ plasmonic...
Post on 31-May-2020
Embed Size (px)
st a tu
Plasmonic Nanopores www.pss-a.com
Plasmonic Nanopore with Nanopattern and Nanoparticles for Single Molecule Analysis
Seong Soo Choi,* Myoung Jin Park, Sae-Joong Oh, Chul Hee Han, Yong-Sang Kim, and Nam Kyou Park
In this report, the nano-hole on the electron beam induced membrane surrounded by periodic groove patterns are fabricated by focused ion beam technique (FIB), field emission scanning electron microscopy (FESEM), and transmission electron microscopy (TEM). Initially, a �200 nm thick Au films was deposited on the microfabricated pyramid, or on the flat plate by using a sputter-deposition technique. Nano-pore formation inside the FIB drilled Au aperture was controlled down to a few nanometer by using electron beam irradiations. Periodic patterns would enhance the optical intensity through the nano-aperture. Au particles were formed on the membrane several months after electron beam irradiations. In addition, surface plasmon- enhanced Raman spectroscopy measurements were performed and the greatest optical intensity from on the pyramidal aperture surrounded with the nanopattern was measured. Fabricated plasmonic pore-device can be utilized as a next generation optical sensor for single molecule analysis. TEM images of the fabricated nanopore surrounded by periodic patterns on the plate are presented with electron beam profile on the detector.
We previously fabricated the nano-hole surrounded with periodic patterns. The optical transmission through the metallic nanometer size single aperture is proportional to (d/λ)4, where d is the diameter and λ is the input wavelength. The transmitted optical intensity through the nano-aperture would be very weak, therefore, the nano-aperture surrounded by periodic patterns was designed, and the enhanced optical intensity is reported.[1–3]
The solid state nanopore device for single molecule analysis is currently fabricated on a thin SiN membrane or a graphene by
Prof. S. S. Choi, Prof. S.-J. Oh, Prof. C. H. Han SunMoon University, Sunmoon-ro, Tangjung myun, 31460, South Korea E-mail: email@example.com; firstname.lastname@example.org
Prof. M. J. Park Korea Military Academy, Nowon-ku, Harang-ro Mailbox 77-1, Seoul, South Korea
Prof. Y.-S. Kim Sungkyunkwan University, Jang-An-ku, Seobu-ro, Suwon 16419, South Korea
Prof. N. K. Park Seoul National University, Shinrim-dong, Kwanak-Gu, Seoul 08826, South Korea
Phys. Status Solidi A 2017, 215, 1700484 © 21700484 (1 of 5)
using high energy TEM electron beam irradiations. However, all of DNA translo- cation experiments are reported to have high error rates with electrical character- izations.[4,5] It may be due to electric dipole layer formation inside the pore channel. Current genome detection techniques are performed under the optical detection technique. Recently, nanoplasmonic sens- ing for surface plasmon resonance based on ordered flow-through nanohole array with its diameters ranging from 300 to 100 nm was reported.[6,7]
However, the nanopore with �10 nm diameter for an optical detection technique has yet to be fabricated. We previously reported fabrication of the nano-aperture surrounded by the periodic patterns on pyramidal probes to improve the low transmittance of light through the nano- size aperture.[8–10] We also have fabricated the nanopore with its diameter ranging from 10 to 3 nm inside the FIB drilled
aperture by using various surface treatments including electron beam irradiations and ion beam irradiation.
Formation of the Au nanoparticle on the diffused membrane during the electron beam processing was also reported.[11–13]
Plasmonic Au nanoparticle can provide the huge optical enhancement of 106-fold increase, so that it can be utilized as surface enhanced Raman spectroscopy (SERS) sensor. We carried out the optical measurements by using SERS technique and observed the highest optical intensity from the aperture surrounded with the periodic nano-pattern on pyramid. The nanopore with periodic groove nano-patterns, along with the Au particles formedon thepore-containingmembranecanbeutilized as a plasmonic optical device for single molecule bio sensor.
2. Experimental Section
2.1. Fabrication Procedure of the Specimen
Au nano-holes with periodic groove patterns on the pyramid, and on the flat plate were also fabricated as presented in Figure 1. The nano-holes on top of the pyramidal structures were fabricated using conventional Si microfabrication process such as photolithography, wet etching, stress-induced thermal oxidation, and metal sputter deposition. The detailed fabrication process is
017 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim
Figure 1. Fabrication process for the microfabricated pyramidal probe array in (a)–(f). FESEM images of the microfabricated (10� 10) pyramid array (g) with a single pyramid (h). Figure 2. Optical intensities (Ixz) and electric fields (Ex) through Au nano-
apertures are shown by using FDTD simulations on the plate and on the pyramid, with and without periodic groove patterns. (X axis: distance, Y axis: arbitrary scale). Optical intensities and electric fields intensities from the samples with periodic groove patterns greater with directionality than the sample without periodic grooves are clearly presented.
st a tu
also given elsewhere.[15,16] The stress-induced thermal oxidation provides the thinner oxide at the apex of the pyramid. After revealing the oxide pyramidal array by using a tetramethylam- monium hydroxide (TMAH) etchant solution, the Au thin film was sputter deposited, followed by drilling nanoholes by using focused ion beam (FIB). The pyramidal array by tuning depth, pitch, and width of the V-groove well can be an excellent SERS substrate due to surface plasmonic effect.
The flat Au plate samples were either fabricated by using plateau pyramid structures, or purchased from commercial company (www.temwindows.com).
2.2. Sample Preparation and Its Characterization
Sample preparation processes were carried out at National Nanofabrication Center (NNFC, Daejeon, South Korea), and Korea Advanced Nano Fab Center (KANC, Suwon, South Korea). Surface modifications with electron beam irradiations by using FESEM and with 30 keV focused Ga ion beam with 1.4 nA were performed with Dual Beam Helios FIB (FEI). High energy electron beam irradiations were carried out by using TEM (JEM- 2010, JEM-3011 HR). Electron beam currents during specimen processing were obtained from electronic control panel display since Faraday cup was not installed for our TEM instruments. However, a big aperture on the specimen with �10 μm diameter were drilled to measure the electron beam currents on the fluorescent disk equipped with TEM instruments. In order to find the influence of the periodic nanopatterns on the optical intensity, 2 dimensional simulations were carried by using a commercial tool (Opti-FDTD, OptiWave).
Figure 3. The peaks of the electric fields for the periodic groove patterns on the plate are shown by FDTD simulation. The diameter of the aperture is 300 nm and the width, the pitch, the depth are 100, 250, and 100 nm, respectively.
2.3. Finite Difference Time Domain (FDTD) Simulation Analysis on the Plate and the Pyramid
Figure 2 shows the finite-difference time-domain (FDTD) simulation results for the four different situations; i) a nano- aperture on the Au plate with a 300nmdiameter with andwithout periodic nanopatterns in (a) and (c); ii) a nano-aperture on top of the Au pyramid with and without periodic patterns in (b) and (d).
Thickness of Au film is set to be 300 nm for both the flat plate and the pyramid. The optical intensities and the electric field
Phys. Status Solidi A 2017, 215, 1700484 1700484 (
through the nano-apertures are presented in the upper column and in the down column, respectively, in Figure 2.
Figure 3 presents the peaks formed on the periodic grooves by using FDTD simulations. The width, the pitch, and the depth of the groove patterns are 100, 250, and 100 nm, respectively. The diameter of the aperture is designed to be 300 nm. Hot spot zone on the main hole at the center and the enhanced optical peaks at the periodic grooves are shown in Figure 3.
2.4. Fabrication of Nano-Holes Surrounded with Periodic Groove Patterns
Periodic groove patterns on the pyramids and on the flat plates were engraved by using 30 keV FIB technique (Dual Beam Helios, FEI). FESEM images were also obtained by utilizing the instrument equipped with Dual BeamHelios FIB as in Figure 4.
© 2017 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim2 of 5)
http://www.temwindows.com http://www.advancedsciencenews.com http://www.pss-a.com
Figure 4. FESEM images of three different types of the patterns drilled on the Au deposited pyramidal structures. Square pattern, circular pattern, and elliptical patterns were drilled on pyramids as in (a), (b), and (c), respectively. The depth, the pitch, and the width is designed to be �100, �250, and 100 nm, respectively.
Figure 6. Electron beam profile on the detector through the groove patterns are shown. A TEM image of a nano-aperture surrounded with 5 groove pattern is inserted (top right).
st a tu
Square patterns and circular groove patterns c